- About this Journal ·
- Abstracting and Indexing ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

ISRN Condensed Matter Physics

Volume 2012 (2012), Article ID 208234, 8 pages

http://dx.doi.org/10.5402/2012/208234

## Cerium-Doped Endohedral Fullerene: A Density-Functional Theory Study

Physics Department, Faculty of Science, King Abdulaziz University, P.O. Box 80203, Jeddah 21589, Saudi Arabia

Received 15 February 2012; Accepted 29 March 2012

Academic Editors: C. Andreani, A. Cantarero, and A. Krimmel

Copyright © 2012 A. Z. AlZahrani. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

First-principles total energy calculations of the structural and electronic properties of Ce-doped fullerene have been performed within the framework of the density functional theory at the generalized gradient approximation level. Among various locations, Ce atom was found to engage with the six-fold carbon ring. The total energy is found to significantly change as the Ce atom being shifted from the center of the cage toward the edge close to the six-membered ring where the total energy reaches its local minimum. Moreover, repulsive interaction between Ce atom and the cage components turns as the adatom directly interacts with the six C atoms of the ring. The lowest-energy CeC_{60} geometry is found to have a binding energy of approximately 5.34 eV, suggesting strong interaction of the dopant with the cage members. Furthermore, fundamental key structural parameters and the total density of states of the optimized structure have been determined and compared with the available data.

#### 1. Introduction

Nowadays, the interest in nanoscale materials has rapidly increased due to their positive use in various technical and scientific researches relating on the energy, environment, and biomedical fields. Carbon is one of the most amazing elements with a vast range of exotic properties. These properties have shed the light on carbon-based nanostructures, such as fullerenes [1], carbon nanotubes [2], and graphene [3]. Since its discovery in 1985 (Nobel Prize in 1996) [1], the subject of fullerene molecule C_{60}, the closed-cage carbon molecules, has attracted immense interest and attention due to its fascinating chemical and physical properties [4–7]. Indeed, the discovery of fullerenes has opened the gate for the production and investigation of much more suitable material building blocks which could be used as drug deliverers in medical applications and/or possible superconductors in technological applications. Therefore, fullerene provides an entirely new branch of chemistry, materials science, and physics. Moreover, solid fullerene is treated as a semiconductor material [8], and its structure is described in the face-centered cubic lattice. Unlike the carbon nanotubes with only hexagonal cells, the fullerene consists of both pentagons and hexagons with two classes of bond lengths: a shorter bond length connecting two successive hexagons and a longer bond length joining a hexagon and pentagon. While the dependence of properties at nanoscale provides an opportunity to test and experiment with various materials, the fullerene is considered as a suitable candidate for nanotechnology since it has the right size and chemical stability. Therefore, the properties of fullerenes can be tuned and enhanced by doping various elements. Depending on the site of doping, fullerenes can be functionalized into three main categories: exohedral fullerenes with the dopant outside the cage, endohedral fullerenes with the dopant inside the cage, and on-site fullerene with the dopant replacing one C atom.

Recently, endohedral fullerene, a member of fullerene family with a dopant encaged within the sphere, has received remarkable attention in various experimental [9–18] and theoretical [19–30] investigations due to its exotic physical and chemical properties such as pseudoatom behavior, magnetism, and superconductivity. The incorporation of lanthanum (La) atom inside the cage of the C_{60} structure has been experimentally investigated by Heath et al. [9] to detect the existence of endohedral metallofullerene complexes. They found, using laser vaporization and mass spectra, that both La and La_{2} form endohedral fullerenes. Later, Shinohara and coworkers have studied the production of yttrium endohedral YC_{60} [10] and scandium endohedral ScC_{60} [11] using arc and laser vaporization of metal-graphite composites in helium atmosphere. Kortan et al. [12] found that a high concentration of calcium (Ca) doped C_{60} experienced phase transitions from face-centered cubic to simple cubic via body-centered cubic. Furthermore, doping of radioactive elements, such as beryllium (Be) [13] and gadolinium (Gd) [14], has been found to be properly encaged inside a C_{60} cluster, leading to substantial applications in nuclear wasting disposal such as nanocontainer radioactivities [31]. Other experimental studies have been reported on the purification of EuC_{60} [15] and ErC_{60} [16] using chemical extraction from carbon soot and high-performance liquid chromatography (HPLC) and investigated the optical properties of purified LiC_{60} [17] using Raman and infrared spectra. Theoretically, the electronic and optical properties of potassium-(K-) doped fullerene [19, 20] have been calculated using the local density approximation (LDA) of the density functional theory (DFT). In their study, Xu et al. [20] have reported that face-centered cubic K_{3}C_{60} has a superconducting nature, whereas body-centered cubic K_{6}C_{60} behaves like an insulator with sufficient agreement with the electron-energy-loss spectra measurements. Saito and Oshiyama [21] studied the electronic structure of Ca_{3}C_{60} and Ca_{5}C_{60} solids. Their calculations revealed electronic charge transfer from Ca 4s states to the lowest-unoccupied state () of the C_{60} cluster and a strong hybridization between the second lowest-unoccupied state () of the C_{60} cluster and the 4s states of the Ca atoms at the off-center position of the octahedral interstitial site. Thereafter, Umemoto and Saito [22] investigated the electronic properties of the superconducting body-centered orthorhombic barium fullerene Ba_{4}C_{60} within the framework of the LDA of the DFT scheme. It has been found that Ba states strongly hybridize with C_{60} states through pentagons faces, leading with the asymmetric lattice to the splitting of the states, and hence, is partially filled. Lu and coworkers [23] have presented *ab initio* investigations for the structural and electronic properties of endohedral beryllium BeC_{60} using the DFT method. Their results show that Be occupies the center of the fullerene cage preserving its atomic electronic configuration. They also found a repulsive interaction between the Be atom and the fullerene cage. Moreover, it has been found that small hydrogenated atoms can also be doped in fullerene. Erkoç and Türker [24–26] have reported, using semiempirical self-consistent field molecular orbital (SCF-MO) method, on the structural and electronic properties of fullerene upon the deposition of hydrogenated B, C, N, Al, Si, and P atoms. It has been found that these endofullerene are stable but endothermic. Using *ab initio* molecular dynamics simulations based on the all-electron mixed-basis approach, Ohtsuki and Ohno [27] have shown that the inclusion of a Po atom into C_{60} through either pentagon or hexagon rings is equally preferable. Very recently, Yang et al. [7] have presented first-principles DFT calculations for the electronic structure of single B-, N-, Co-, P-, and Bi-doped C_{60} solids. Also they have reproduced the calculations for two and three Bi atoms in C_{60} solids. For a single dopant concentration, they have found that B-, P-, and Co-doped C_{60} solids are *n*-type semiconductors, whereas N doped C_{60} solid is a *p*-type semiconductor. For two and three Bi atoms in C_{60} solids, the resultant structures are a *p*-type semiconductor and metal, respectively. Despite much available experimental and theoretical investigations of endohedral fullerenes, there is a lack of theoretical studies of endohedral fullerene doped by rare earth metals with unfilled shells. In the present work, we will report on the structural and electronic properties of Ce-doped C_{60} solids using DFT.

#### 2. Theoretical Framework

Density-functional theory calculations employing the self-consistent Kohn-Sham functional were performed using the Vienna *ab initio* simulation package (VASP) [32–35]. The single-particle Kohn-Sham wave functions [36] were expanded using plane waves basis sets up to cut off energy of 20 Ry. The charge density cutoff energy was set to 80 Ry. We treated the electron-ion interactions using the ultrasoft pseudopotential [37]. The Perdew-Burke-Ernzerhof exchange-correlation scheme [38] was considered to take into account the electron-electron interactions. Self-consistent solutions of the Kohn-Sham equations were obtained by employing a Monkhorst-Pack [39] grid of **k**-points for the integration over the Brillouin zone. The full electronic density of states was also calculated with a high **k**-point sampling of . The relative tolerance in the density matrix, taken as self-consistent field (SCF) convergence criterion, was set to 10^{−5} eV. Relaxed atomic positions were obtained by using the total energy and force minimization methods. The force tolerance in the minimization procedure was set to approximately 0.005 eV/Å, in which no explicit symmetry constraints were imposed during the minimization.

#### 3. Results and Discussion

The structural and electronic properties of the fcc fullerene have been determined to thoroughly investigate the modification of the fullerene upon the doping of Ce atom. Before presenting results for fullerene and Ce-doped fullerene, energy convergence tests with respect to the lattice constant, kinetic energy cut off, and special **k**-points were performed. Our calculations indicate that a minimum total energy value is obtained for a lattice parameter of 27.03 Bohr (14.30 Å) as shown in Figure 1. This value is slightly overestimated comparing with the experimental value of 14.17 Å [40, 41] but is in good agreement with previously reported value of 14.29 Å along the orientation [42]. In their study, Zólyomi et al. [42] have shown that the orientational effects play a significant role in determining the lattice constant of C_{60}-based molecular crystals.

It is also clear from Figure 2 that very well-converged total energy values can be achieved for energy cutoff values of 20 Ry or higher.

Similarly, the choice of 6 special **k**-points (within Monkhorst-Pack grid) for self-consistent calculation of charge density is also found to be quite acceptable. Increasing the special** k**-points to 24 (within Monkhorst-Pack grid) only decreases the total energy by 0.02 eV/cell. Figure 3 shows the relaxed geometry of the C_{60} configuration. It is found that the bond length of the hexagon-pentagon (6-5) is approximately C_{1}–C_{2} = 1.465 Å, while the C_{3}–C_{4} = 1.41 Å for a hexagon-hexagon (6-6), suggesting quite agreement with the neutron diffraction measurements [43] of 1.46 and 1.39 Å, respectively.

These values are in the range of the double of the covalent radius of the carbon atom. Moreover, it is quite identical to the calculated C–C bond length of diamond (1.52 Å) and graphite (1.42 Å). This, therefore, indicates wide range of similarity in the structural behavior of fullerene with the other C-based compounds. Furthermore, the inner and outer diameters of the ball are found to be 3.52 and 10.28 Å, respectively, indicating a mean ball diameter of 6.9 Å. These values are quite close to the previously reported values.

To investigate the fundamental electronic properties of fullerene, we have performed the electronic density of states (DOS) for fcc C_{60} as depicted in Figure 4. It is clearly shown that the energy band is approximately 1.57 eV, which is larger than the calculated band gap of 1.34 eV obtained by Ching et al. [19]. Furthermore, it is noted that both the valence states and the conduction states consist of a number of small fragments. The origin of the occupied peaks is mainly due to the *p* states of the C atoms with little contributions from the carbon* s* orbitals. These filled states are quite narrow and separated by very small gaps. Such a form of localized states is a fundamental feature of molecular-like structures.

The total charge density plot of the relaxed atomic structure of fullerene is plotted in a plane passing through the center of fullerene, as shown in panel (a) of Figure 5. It is clearly shown that the charge is entirely accommodated around the five- and six-folded carbon atoms, indicating that fullerene has a similar charge distribution as the graphite and diamond structures with a *sp ^{3}* covalent bond formation. Moreover, the partial charge density plots of the highest occupied and lowest unoccupied states of the fullerene are also presented in panels (b) and (c) of Figure 5, respectively. These planar plots are performed along the plane at the Γ point of the Brillouin zone with an origin being chosen at the center of the ball. Figure 5 (b) shows that the highest occupied states mainly originate from the -orbitals of the six-folded carbon atoms. The lowest unoccupied states are largely nature around the six-folded carbon atoms as shown in (c).

Having discussed the fundamental properties of the clean fullerene, we now are ready to investigate the effect of incorporation of Ce atom in the fullerene. To the best of our knowledge, the modification of the structural and electronic properties of C_{60} fullerene upon the doping of Ce atom is not yet established. So far, there is no direct information about the exact geometry of Ce-doped fullerene, and we have used our *ab initio* density functional calculations to optimize the adsorption site of a single Ce adatom on the fullerene unit cell. To achieve such a purpose, five different initial positions taking into account all the symmetry sites and spanning uniformly the unit cell have been investigated, as shown in Figure 6. These doping sites are based on a single Ce atom placed (a) at the origin, (b) in a direct interact with the hexagon, (c) in a direct interact with the pentagon, (d) substituting one carbon atom, and (e) above the common C–C bond connecting two consecutive-hexagon and pentagon.

Unlike the encapsulated N and noble gas atoms [44–47] and metallic atoms like Be, Ca, Li, Y, La, and Sc [23, 48–51], which all occupy the center or slightly positioned off-center of the fullerene, the absolute minimum corresponding to the lowest total energy has been found for Ce interacting directly with the six-folded ring of the fullerene, as indicated in panel (b) of Figure 6. It is also noted that during the optimization process, the Ce atom that was initially placed elsewhere inside the cage migrates to the six-membered ring. Our total energy calculation suggests that the total energy significantly changes as the Ce atom is shifted from the center of the cage toward the edge close to the hexagonal ring where the total energy reaches its local minimum, as shown in Figure 7. The interaction between Ce and the cage turns to be repulsive as the Ce atom directly interacts with the C atoms of the ring.

However, this optimal structure indicates that the CeC_{60} in its symmetry is the ground state. The binding energy of such a structure is determined to be 5.34 eV, which is smaller than the value obtained for CeC_{82} of 6.696 eV. However, this value is greater than the values of 2.65, 3.77, and 4.29 eV obtained for Gd, La, and PoC_{60}, respectively. The calculated value of binding energy indicates, though it is smaller than that of CeC_{82}, a strong interaction of Ce and states with the states of the C atoms. With respect to the fully relaxed pure fullerene, the optimized hexagon-hexagon and hexagon-pentagon C–C bond lengths of the CeC_{60} are found to be slightly elongated by an approximately 0.0015 and 0.002 Å, respectively. These observations have also been seen in some metallic dopant in fullerene (see, e.g., [22, 23]), suggesting possible charge transfer from the Ce atom to the C atoms. Despite that the structural change of the CeC_{60} is only a few decimals, it is vital to the ground state energy calculation. The average Ce–C bond length is calculated to be 2.52 Å, which is almost equivalent to the sum of their covalent radii, indicating a strong bond formation. Consistent with the values obtained for pure fullerene, the inner and outer radii of the cage remain unaltered, suggesting that Ce does not distort the overall structure of the ball but a little appreciable elongation in the double and single C–C bond of the cage rings as discussed earlier. Finally, we have calculated the average C–Ce–C bond angle of approximately 56.12°. It has also been calculated for NiC_{60} [52] that the drop shape is further characterized by the deviation from planarity of approximately 56.8°.

The electronic band structure of the endohedral Ce-doped fullerene along the symmetry direction of the face-centered cubic Brillouin zone is depicted in Figure 8. At the Γ point, it is clearly shown that the energy gap of the pure fullerene has been significantly reduced to approximately 0.2 eV due to the quite strong interaction between the dopant and the carbon species. The highest occupied state slightly crosses the Fermi level at both L and K points of the Brillouin zone. We have noticed that the highest occupied state is quite straight along the ΓX direction, indicating that this state originates from the Ce-filled orbitals. Similarly, the lowest unoccupied state is rather straight along the LX direction, suggesting a long-range interaction between the dopant and the host material.

To investigate the density distribution of the present system, we have plotted DOS. Figure 9 shows that the overall electronic structure of the system is metallic. Although there are no appreciable changes in the valence region of the Ce-doped fullerene comparing with the clean fullerene, significant changes can be clearly observed in the energy interval to + 2.5 eV. A new shoulder S_{1} has been created in the vicinity of the fullerene band gap and slightly below the Fermi level. This shoulder, however, is believed to be originated from the 5*d* orbital of the Ce atom. A well-developed peak is also observed at about + 1.8 eV, which is partially contributed by the states of the Ce atom. At approximately + 5.0 eV, the undeveloped peak observed for fullerene has now been a well-defined peak. Overall, the narrow peaks seen in pure fullerene are now slightly broadened upon the doping of the Ce atom with minor contribution from Ce 4*f* electrons to the metallic ground state of the system.

To elucidate the nature of the Ce–C bonding formation, we have plotted the total charge density along a line joining the Ce atom with its nearest neighbors. Our results, plotted in Figure 10, indicate that the charge is strongly localized around the C atoms with little amount of charge being accommodated around the dopant, suggesting an ionic nature for the C–Ce bond. We also conclude that a large amount of charge has been transferred from the Ce atom to its nearest neighbor C atoms due to its electronegativity. To estimate the value of the transferring charges, we employed a simple scheme in which we calculate total charge of the total charge density in a sphere, around a Ce atom, of radius equivalent to half the distance between the Ce atom and the nearest C atom. Following a similar method with the exact size of the studied unit cell (fullerene cell), the charge density around an isolated Ce atom is calculated. Using the numerical results from these two calculations, approximately 0.64e charge has been transferred from the Ce atom to its neighboring C atoms. The Ce-to-C_{60} charge transfer, therefore, is responsible for an almost perfect alignment between (6,6) and (6,5) C–C bonds.

A summary of the structural and electronic parameters of CeC_{60} compared with other endohedral metal-doped C_{60} is presented in Table 1.

#### 4. Summary

Using *ab initio* density functional calculations, the structural and electronic properties of Ce-doped fullerene have been investigated. It is found that the ground-state structure of CeC_{60} composes of a Ce atom bonded to the hexagonal ring of the cage with a binding energy of approximately 5.34 eV. The structure is semiconducting at the Γ point with a significant reduction in the fullerene band gap. The C–Ce bond is found to be of an ionic nature with a large amount of charge being transferred from the Ce to the C atoms. Upon the charge transfer from the Ce to C atoms, the double and single C–C bonds have been slightly elongated.

#### Acknowledgment

The financial support (project no. 66/130/1431) from the deanship of scientific research (DSR) at King Abdulaziz University (KAU) is highly appreciated and gratefully acknowledged.

#### References

- H. W. Kroto, J. R. Heath, S. C. O'Brien, R. F. Curl, and R. E. Smalley, “C
_{60}: buckminsterfullerene,”*Nature*, vol. 318, no. 6042, pp. 162–163, 1985. View at Publisher · View at Google Scholar · View at Scopus - S. Iijima, “Helical microtubules of graphitic carbon,”
*Nature*, vol. 354, no. 6348, pp. 56–58, 1991. View at Scopus - K. S. Novoselov, A. K. Geim, S. V. Morozov et al., “Electric field in atomically thin carbon films,”
*Science*, vol. 306, no. 5696, pp. 666–669, 2004. View at Publisher · View at Google Scholar · View at Scopus - T. A. Spurlin and A. A. Gewirth, “Effect of C
_{60}on solid supported lipid bilayers,”*Nano Letters*, vol. 7, no. 2, pp. 531–535, 2007. View at Publisher · View at Google Scholar · View at Scopus - D. Boawan, N. Thomwattana, and J. M. Hill, “Encapsulation of C
_{60}fullerenes into single-walled carbon nanotubes: fundamental mechanical principles and conventional applied mathematical modeling,”*Physical Review B*, vol. 76, no. 15, Article ID 155411, 8 pages, 2007. View at Publisher · View at Google Scholar - Q. Wang, “Torsional instability of carbon nanotubes encapsulating C
_{60}fullerenes,”*Carbon*, vol. 47, no. 2, pp. 507–512, 2009. View at Publisher · View at Google Scholar · View at Scopus - S. Yang, S. Guo, S. Bai, E. Khosravi, G. L. Zhao, and D. Bagayoko, “Doped C
_{60}study from first principles simulation,”*Journal of Superconductivity and Novel Magnetism*, vol. 23, no. 6, pp. 877–880, 2010. View at Publisher · View at Google Scholar · View at Scopus - S. Saito and A. Oshiyama, “Cohesive mechanism and energy bands of solid C
_{60},”*Physical Review Letters*, vol. 66, no. 20, pp. 2637–2640, 1991. View at Publisher · View at Google Scholar · View at Scopus - J. R. Heath, S. C. O'Brien, Q. Zhang et al., “Lanthanum complexes of spheroidal carbon shells,”
*Journal of the American Chemical Society*, vol. 107, no. 25, pp. 7779–7780, 1985. View at Scopus - H. Shinohara, H. Sato, Y. Saito, M. Ohkohchi, and Y. Ando, “Mass spectroscopic and ESR characterization of soluble yttrium-containing metallofullerenes YC
_{82}and Y_{2}C_{82},”*Journal of Physical Chemistry*, vol. 96, no. 9, pp. 3571–3573, 1992. View at Scopus - H. Shinohara, H. Sato, M. Ohkohchi et al., “Encapsulation of a scandium trimer in C
_{82},”*Nature*, vol. 357, no. 6373, pp. 52–54, 1992. View at Scopus - A. R. Kortan, N. Kopylov, S. Glarum et al., “Superconductivity at 8.4 K in calcium-doped C
_{60},”*Nature*, vol. 355, no. 6360, pp. 529–532, 1992. View at Scopus - T. Ohtsuki, K. Masumoto, K. Ohno et al., “Insertion of Be atoms in C
_{60}fullerene cages: Be@C_{60},”*Physical Review Letters*, vol. 77, no. 17, pp. 3522–3524, 1996. View at Scopus - Y. Kubozono, H. Maeda, Y. Takabayashi et al., “Isolation and characterization of C
_{60},”*Journal of the American Chemical Society*, vol. 118, no. 29, pp. 6998–6999, 1996. View at Publisher · View at Google Scholar · View at Scopus - T. Inoue, Y. Kubozono, S. Kashino et al., “Electronic structure of Eu@C
_{60}studied by XANES and UV-VIS absorption spectra,”*Chemical Physics Letters*, vol. 316, no. 5-6, pp. 381–386, 2000. View at Scopus - T. Ogawa, T. Sugai, and H. Shinohara, “Isolation and characterization of Er@C
_{60},”*Journal of the American Chemical Society*, vol. 122, no. 14, pp. 3538–3539, 2000. View at Publisher · View at Google Scholar · View at Scopus - A. Gromov, N. Krawez, A. Lassesson, D. I. Ostrovskii, and E. E. B. Campbell, “Optical properties of endohedral Li@C
_{60},”*Current Applied Physics*, vol. 2, no. 2, pp. 51–55, 2002. View at Scopus - R. Klingeler, C. Breuer, I. Wirth et al., “Scanning tunneling spectroscopy of small Ce-doped endohedral fullerenes on HOPG,”
*Surface Science*, vol. 553, no. 1–3, pp. 95–104, 2004. View at Publisher · View at Google Scholar · View at Scopus - W. Y. Ching, M. Z. Huang, Y. N. Xu, W. G. Harter, and F. T. Chan, “First-principles calculation of optical properties of C
_{60}in the fcc lattice,”*Physical Review Letters*, vol. 67, no. 15, pp. 2045–2048, 1991. View at Publisher · View at Google Scholar · View at Scopus - Y. N. Xu, M. Z. Huang, and W. Y. Ching, “Optical properties of superconducting K
_{3}C_{60}and insulating K_{6}C_{60},”*Physical Review B*, vol. 44, no. 23, pp. 13171–13174, 1991. View at Publisher · View at Google Scholar · View at Scopus - S. Saito and A. Oshiyama, “Electronic structure of calcium-doped C
_{60},”*Solid State Communications*, vol. 83, no. 2, pp. 107–110, 1992. View at Scopus - K. Umemoto and S. Saito, “Electronic structure of the Ba
_{4}C_{60}superconductor,”*Physical Review B*, vol. 61, no. 20, pp. 14204–14208, 2000. View at Scopus - J. Lu, Y. Zhou, X. Zhang, and X. Zhao, “Density functional theory studies of beryllium-doped endohedral fullerene Be@C
_{60}: on center displacement of beryllium inside the C_{60}cage,”*Chemical Physics Letters*, vol. 352, no. 1-2, pp. 8–11, 2002. View at Publisher · View at Google Scholar · View at Scopus - Ş. Erkoç and L. Türker, “Structural and electronic properties of endofullerenes X@C
_{60},”*Journal of Molecular Structure*, vol. 634, pp. 195–199, 2003. View at Publisher · View at Google Scholar · View at Scopus - Ş. Erkoç and L. Türker, “AM1 treatment of endohedrally hydrogen doped fullerene,
*n*H_{2}@C_{60},”*Journal of Molecular Structure*, vol. 638, pp. 37–40, 2003. View at Publisher · View at Google Scholar · View at Scopus - Ş. Erkoç and L. Türker, “Ammonia deposition in fullerene: (NH
_{3})*n*@C_{60},”*Journal of Molecular Structure*, vol. 640, pp. 57–61, 2003. View at Publisher · View at Google Scholar · View at Scopus - T. Ohtsuki and K. Ohno, “Formation of Po@C
_{60},”*Physical Review B*, vol. 72, no. 15, Article ID 153411, 3 pages, 2005. View at Publisher · View at Google Scholar · View at Scopus - H. Dodziuk, “Modeling complexes of H
_{2}molecules in fullerenes,”*Chemical Physics Letters*, vol. 410, no. 1–3, pp. 39–41, 2005. View at Publisher · View at Google Scholar · View at Scopus - M. Chi, P. Han, X. Fang, W. Jia, X. Liu, and B. Xu, “Density functional theory of Polonium-doped endohedral fullerenes Po@C
_{60},”*Journal of Molecular Structure*, vol. 807, no. 1–3, pp. 121–124, 2007. View at Publisher · View at Google Scholar · View at Scopus - G. Li, R. F. Sabirianov, J. Lu, X. C. Zeng, and W. N. Mei, “Electronic and magnetic properties of endohedrally doped fullerene Mn@ C
_{60}: a total energy study,”*Journal of Chemical Physics*, vol. 128, no. 7, Article ID 074304, 6 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - I. Amato, “Researchers swap material evidence in Boston,”
*Science*, vol. 258, no. 5090, pp. 1886–1887, 1992. View at Scopus - G. Kresse and J. Hafner, “Ab initio molecular dynamics for liquid metals,”
*Physical Review B*, vol. 47, no. 1, pp. 558–561, 1993. View at Publisher · View at Google Scholar · View at Scopus - G. Kresse and J. Furthmüller, “Efficiency of ab-initio total energy calculations for metals and semiconductors using a plane-wave basis set,”
*Computational Materials Science*, vol. 6, no. 1, pp. 15–50, 1996. View at Publisher · View at Google Scholar · View at Scopus - G. Kresse and D. Joubert, “From ultrasoft pseudopotentials to the projector augmented-wave method,”
*Physical Review B*, vol. 59, no. 3, pp. 1758–1775, 1999. View at Scopus - G. Kresse and J. Furthmüller, “Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set,”
*Physical Review B*, vol. 54, no. 16, pp. 11169–11186, 1996. View at Scopus - W. Kohn and L. J. Sham, “Self-consistent equations including exchange and correlation effects,”
*Physical Review A*, vol. 140, no. 4, pp. A1133–A1138, 1965. View at Publisher · View at Google Scholar · View at Scopus - D. Vanderbilt, “Soft self-consistent pseudopotentials in a generalized eigenvalue formalism,”
*Physical Review B*, vol. 41, no. 11, pp. 7892–7895, 1990. View at Publisher · View at Google Scholar · View at Scopus - J. P. Perdew and A. Zunger, “Self-interaction correction to density-functional approximations for many-electron systems,”
*Physical Review B*, vol. 23, no. 10, pp. 5048–5079, 1981. View at Publisher · View at Google Scholar · View at Scopus - H. J. Monkhorst and J. D. Pack, “Special points for Brillouin-zone integrations,”
*Physical Review B*, vol. 13, no. 12, pp. 5188–5192, 1976. View at Publisher · View at Google Scholar · View at Scopus - M. S. Dresselhaus, G. Dresselhaus, and P. C. Eklund,
*Science of Fullerenes and Carbon Nanotubes*, Academic Press, San Diego, Calif, USA, 1996. - S. Pekker, E. Kováts, G. Oszlányi et al., “Rotor-stator molecular crystals of fullerenes with cubane,”
*Nature Materials*, vol. 4, no. 10, pp. 764–767, 2005. View at Publisher · View at Google Scholar · View at Scopus - V. Zólyomi, J. Koltai, J. Kürti, and S. Pekker, “Theoretical study of the electronic structure of fullerene-cubane cocrystals,”
*Physical Review B*, vol. 78, no. 11, Article ID 115405, 6 pages, 2008. View at Publisher · View at Google Scholar · View at Scopus - W. I. F. David, R. M. Ibberson, J. C. Matthewman et al., “Crystal structure and bonding of ordered C
_{60},”*Nature*, vol. 353, no. 6340, pp. 147–149, 1991. View at Scopus - H. Mauser, N. J. R. V. Hommes, T. Clark et al., “Stabilization of atomic nitrogen inside C
_{60},”*Angewandte Chemie*, vol. 36, no. 24, pp. 2835–2838, 1997. View at Scopus - A. Weidinger, M. Waiblinger, B. Pietzak, and T. Almeida Murphy, “Atomic nitrogen in C
_{60}:N@C_{60},”*Applied Physics A*, vol. 66, no. 3, pp. 287–292, 1998. View at Scopus - L. Pang and F. Brisse, “Endohedral energies and translation of fullerene-noble gas clusters G@Cn (G = helium, neon, argon, krypton and xenon; $n=60$ and 70),”
*Journal of Physical Chemistry*, vol. 97, no. 33, pp. 8562–8563, 1997. View at Publisher · View at Google Scholar - M. Son and Y. K. Sung, “The atom-atom potential. Exohedral and endohedral complexation energies of complexes of X@C
_{60}between fullerene and rare-gas atoms (X = He, Ne, Ar, Kr, and Xe),”*Chemical Physics Letters*, vol. 245, no. 1, pp. 113–118, 1995. View at Publisher · View at Google Scholar - L. S. Wang, J. M. Alford, Y. Chai et al., “The electronic structure of Ca@C
_{60},”*Chemical Physics Letters*, vol. 207, no. 4–6, pp. 354–359, 1993. View at Scopus - W. Andreoni and A. Curioni, “Ab initio approach to the structure and dynamics of metallofullerenes,”
*Applied Physics A*, vol. 66, no. 3, pp. 299–306, 1998. View at Scopus - W. Andreoni and A. Curioni, “Freedom and constraints of a metal atom encapsulated in fullerene cages,”
*Physical Review Letters*, vol. 77, no. 5, pp. 834–837, 1996. View at Scopus - T. Guo, G. K. Odom, and G. E. Scuseria, “Electronic structure of Sc@C
_{60}: an ab initio theoretical study,”*Journal of Physical Chemistry*, vol. 98, no. 32, pp. 7745–7747, 1994. View at Scopus - E. Neyts, A. Maeyens, G. Pourtois, and A. Bogaerts, “A density-functional theory simulation of the formation of Ni-doped fullerenes by ion implantation,”
*Carbon*, vol. 49, no. 3, pp. 1013–1017, 2011. View at Publisher · View at Google Scholar · View at Scopus